EFFECTS OF AT-HOME AND IN-OFFICE
BLEACHING ON THE SHEAR BOND STRENGTH OF
METAL, CERAMIC AND COMPOSITE BRACKETS TO
ENAMEL – AN IN VITRO STUDY
Dissertation submitted to
The Tamil Nadu Dr M.G.R. Medical University
In partial fulfillment of the degree of
MASTER OF DENTAL SURGERY
ORTHODONTICS AND DENTOFACIAL ORTHOPEDICS
This is to certify that the dissertation entitled “
EFFECTS OF AT-HOME AND
IN-OFFICE BLEACHING ON THE SHEAR BOND STRENGTH OF
METAL, CERAMIC AND COMPOSITE BRACKETS TO ENAMEL
– AN IN VITRO STUDY” is a bonafide research work done by Dr. RAHUL. M, postgraduate student during the period of 2012-2015 under my guidance and supervision. This dissertation is submitted to the Tamil Nadu Dr M.G.R Medical University, Chennai in partial fulfillment of the requirements for the award of Master of Dental Surgery, Branch V (Orthodontics and Dentofacial Orthopedics). It has not been submitted (partially or fully) for the award of any other degree or diploma.
Dr. P. Anilkumar MDS Dr. Amal. S. Nair MDS
Professor & Head of the Department, Reader,
Department of Orthodontics Department of Orthodontics & Dentofacial Orthopedics & Dentofacial Orthopedics, Sree Mookambika Institute Sree Mookambika Institute Of Dental Sciences, of Dental Sciences,
SREE MOOKAMBIKA INSTITUTE OF DENTAL SCIENCES
ENDORSEMENT BY THE PRINCIPAL / HEAD OF THE INSTITUTION
This is to certify that the dissertation entitled “EFFECTS OF AT-HOME AND IN-OFFICE BLEACHING ON THE SHEAR BOND STRENGTH OF METAL, CERAMIC AND COMPOSITE BRACKETS TO ENAMEL – AN INVITRO STUDY” is a bonafide research work done by Dr. RAHUL. M under the guidance of
Dr. P. Anil Kumar MDS, Professor and Head, Department of Orthodontics and Dentofacial Orthopedics, Sree Mookambika Institute of Dental Sciences, Kulasekharam.
Date: DR. ELIZABETH KOSHI MDS,
I would like to sincerely thank Dr. Anilkumar. P, Professor and Head of the Department, Department of Orthodontics, Sree Mookambika Institute Of Dental Sciences, Kulasekharam for his guidance, understanding and most importantly his patience during my course. His mentorship was paramount in providing a well rounded experience which helped me in attaining my goals. I believe that his actions provided me with the unique opportunity to gain a wider breadth of experience and knowledge. For everything you’ve done for me, I thank you.
I would also like to thank my former head of the department,
Dr.G.Rajasekhar from the bottom of my heart for filling my mind with confidence and energy. I bow my head in acknowledgement for your love and support.
I consider it a great privilege and an honour to express my profound gratitude to Dr.Shino.P.Mathew, Professor, Department of Orthodontics, SMIDS, Kulasekharam for his guidance. He encouraged me to not only grow as an experimentalist but also as an independent thinker. I have benefited greatly from his attention to the finer details.
I thank Dr.Amal.S.Nair, Reader, Department of Orthodontics, SMIDS, Kulasekharam for providing me his great insights, advices, help and kind support right from the selection of my thesis topic through out the course of this study.
I sincerely thank Dr. Anna Oommen, Senior Lecturer, SMIDS, Kulasekharam. She had always supported me whenever I was in need. Thank you so much for sharing your experience.
I would also like to thank my seniors Dr. Rajesh, Dr. Anjana, fellow post graduate student Dr. Rajkumar. R and my juniors Dr. Anitha, Dr. Smitha, Dr. Harsha and Dr. Thasneem for their constant encouragement and help.
I would like to extend my gratefulness to my parents and friends for their unconditioned love and support.
LIST OF ABBREVIATIONS i
LIST OF FIGURES ii – iii
LIST OF TABLES iv
LIST OF GRAPHS v
LIST OF ANNEXURES vi
ABSTRACT vii - viii
AIMS & OBJECTIVES 5
REVIEW OF LITERATURE 6-23
MATERIALS & METHODS 24-30
SUMMARY & CONCLUSION 51-52
BIBILIOGRAPHY ix - xx
LIST OF ABBREVIATIONS
ANOVA Analysis of Variance
ADA American Dental Association
ie That is
LED Light Emitting Diode
MPa Mega Pascals
PF Potassium nitrate and Fluoride
SD Standard Deviation
SEM Scanning Electron Microscopy
LIST OF FIGURES Figure Number Details
Figure 1 Premolars mounted in acrylic blocks
Figure 2 Representative sample of brackets
Figure 3 Armamentarium
Figure 4 Group I samples – control
Figure 5 Group II samples for at-home bleaching
Figure 6 Group III samples for in-office bleaching
Figure 7 Application of in-office bleaching bleaching
Figure 8 Application of at-home bleaching agent
Figure 9 Group II samples after application of at-home bleaching agent
Figure 10 Group III samples after application of in-office bleaching agent
Figure 11 Scanning Electron Microscope
Figure 12 Sputter coating unit
Figure 13 Sputter coated samples
Figure 14 Group I after bonding
Figure 15 Group II after bonding
Figure 16 Group III after bonding
Figure 17 INSTRON machine
iii Figure 19 Shear bond testing (lateral view)
Figure 20 Normal enamel surface (1500X)
Figure 21 Normal enamel surface (3000X)
Figure 22 37 % Phosphoric acid etched enamel surface (1500X)
Figure 23 37 % Phosphoric acid etched enamel surface (3000X)
Figure 24 At-home bleached enamel surface (1500X)
Figure 25 At-home bleached enamel surface (3000X)
Figure 26 In-office bleached enamel surface (1500X)
Figure 27 In-office bleached enamel surface (3000X)
Figure 28 Etched enamel surface after at-home bleaching (1500X)
Figure 29 Etched enamel surface after at-home bleaching (3000X)
Figure 30 Etched enamel surface after in-office bleaching (1500X)
LIST OF TABLES Table
Table-1 Shear bond strength (MPa) values of different samples of group I
Table-2 Shear bond strength (MPa) values of different samples of group II
Table-3 Shear bond strength (MPa) values of different samples of group III
Table-4 Mean values of shear bond strength (MPa) of group I
Table-5 Mean values of shear bond strength (MPa) of group II
Table-6 Mean values of shear bond strength MPa) of group III
Table-7 Multiple comparison of mean shear bond strength (Mpa) with in group I
Table-8 Multiple comparison of mean shear bond strength (Mpa) with in group II
Table-9 Multiple comparison of mean shear bond strength (Mpa) with in group III
Table-10 Multiple comparison of mean shear bond strength (MPa) values of different groups
Table-11 Multiple comparison of mean shear bond strength (MPa) values of different groups
LIST OF GRAPHS
Graph Number Details
Graph I Mean values of shear bond strength (MPa) values of group-I
Graph II Mean values of shear bond strength (MPa) values of group-II
Graph III Mean values of shear bond strength (MPa) values of group-III
Graph IV Multiple comparisons of mean values of shear bond strength (MPa) of different groups
Graph V Multiple comparisons of mean values of shear bond strength (MPa) of different groups
Annexure number Details
1 Institutional Research Committee Certificate
2 Institutional Human Ethics Committee Certificate
The purpose of this in vitro study is to evaluate the effects of at-home and in-office bleaching on the shear bond strength of metal, ceramic and composite orthodontic brackets; and to compare the shear bond strengths of metal, ceramic and composite brackets after at-home and in-office bleaching.
96 human lower premolar teeth were used for this study. 6 teeth were used for SEM study while the remaining 90 were divided into 3 equal groups. Each group was further subdivided into 3 sub groups with 10 samples each. Three protocols were used. In the at-home bleaching group (n = 30), Opalescence non PF bleaching agent (Ultradent, South Jordan, Utah), which contains 10% carbamide peroxide, was applied onto the teeth daily for 14 days and left for 8 hours each day. Teeth in the in-office group (n = 30) were treated with Opalescence boost PF (Ultradent, South Jordan, Utah), which contains 40% hydrogen peroxide gel. These teeth were treated twice in consecutive days. After bleaching, the specimens were stored in distilled water for one day before bonding. Shear bond strength testing was performed on all teeth using universal testing machine, Instron.
viii (IIIa). The mean shear bond strength of ceramic brackets in control group (Ib) was found to be 20.21±0.94 MPa. It decreased to 18.31±1.23 MPa in the at-home bleached (IIb) group and reduced further to 16.13±2.67 MPa in the in-office bleached group (IIIb). The mean shear bond strength of composite brackets in control group (Ic) was found to be 9.81±0.61 MPa. It decreased to 8.06±1.88 MPa in the at-home bleached (IIc) group and reduced further to 7.22±2.15 MPa in the in-office bleached group (IIIc).
The results showed that at-home bleaching did not affect the shear bond strength significantly whereas in-office bleaching reduced shear bond strength of metal, ceramic and composite brackets significantly. It is preferable to use metal or ceramic brackets than composite brackets for bonding 24 hours after bleaching.
1 Beauty or the general appearance of a person is given a lot of importance in the society. Facial appearance plays the most important part in deciding the beauty of a person. While the eyes may be the window to the soul, the mouth is also a window to the body’s physical and mental health.(1) A good smile with well aligned and lighter teeth is considered aesthetic. Realising this, people are constantly striving to improve their smile and in general the appearance of their face since antiquity. The negative effect on psychic and social well being from dentofacial disfigurement is well documented, and it is clear that this is why most patients seek orthodontic treatment. That is why motivation, is stronger in patients with the more severe deviations from the norm.
Perceived improvement of facial esthetics or cosmetic change may be the
main reason why patients and parents seek orthodontic treatment, rather than an
improvement in function that could be of secondary importance to patients. Most
patients view orthodontic treatment as a means to improve dentofacial esthetics.(2)
Significant changes are observed daily in people's self-esteem through minor or major
orthodontic correction. These positive changes can have a significant impact in
people's day today lives. During orthodontic pretreatment consultation, patients as
well as parents frequently express their view on their inhibition towards a natural
smile because of the malalignment or unaesthetic appearance of their dentition.
2 teeth, acid etching, and dental bleaching.
Discoloration of teeth is one of the biggest aesthetic concerns of dental patients. Tooth discoloration may be classified as intrinsic, extrinsic, or a combination of both (3). Intrinsic discoloration is caused by incorporation of chromatogenic material into dentin and enamel during odontogenesis or after eruption.(4) Vital and non-vital bleaching with various whitening agents has now gained worldwide acceptance among clinicians and patients for lightening teeth. However, changes in enamel structure and composition induced by these bleaching agents may decrease the shear bond strength (SBS) of orthodontic brackets.(5).
Orthodontic patients, including a growing population of adults, not only want an improved smile, but they are also increasingly demanding better aesthetics during treatment.(6)Also such patients also expect their orthodontic treatment to go unnoticed or as inconspicuous as possible.
So the options available for them are aesthetic brackets, lingual orthodontics or invisalign.(6) Among these aesthetic brackets are comparatively cheaper to the other options; composite or plastic brackets being so much cheaper than the ceramic brackets.
3 During the 1990’s, manufacturers came up with reinforced plastic brackets
also known as composite brackets, i.e. ceramic reinforced, fiberglass reinforced, and metal slot reinforced polycarbonate brackets, with claims of essentially no adverse clinical effects.(8) The composite bracket used in the current study is Silkon plus, American Orthodontics which is Ca-Al-silicate fibre glass reinforced polycarbonate.(9)
Ceramic brackets were introduced in the 1980’s, and offer many advantages over the then popular traditional aesthetic appliances. Ceramic brackets provide higher strength, more resistance to wear and deformation, better colour stability and, most important to the patient superior aesthetics. All currently available ceramic brackets are composed of aluminium oxide in one of two forms: polycrystalline or monocrystalline.
Polycrystalline zirconia brackets (ZrO2), which reportedly have the greatest
toughness amongst all ceramics, have been offered as an alternative to alumina ceramic brackets.(10) The most apparent difference between the two is their optical clarity: monocrystalline ceramic brackets being noticeably more translucent. The majority of the currently available ceramic brackets rely solely on mechanical retention to prevent enamel damage during debonding.
With an increasing demand for adult orthodontics, orthodontists often encounter patients who are unsatisfied not only with the alignment but also with the color of their teeth (11).
Today, patients can have tooth bleaching done in 2 ways: either in-office or at home bleaching. The most commonly used tooth bleaching agents contain hydrogen
peroxide as the active ingredient. (12)
4 produced by a chemical reaction from sodium perborate or carbamide peroxide. Hydrogen peroxide acts as a strong oxidizing agent through the formation of reactive oxygen molecules; these reactive molecules attack long-chained, dark- colored chromophore molecules and split them into smaller, less colored, and more diffusible molecules (4).
After evaluating the effect of aqueous solutions of hydrogen peroxide at concentrations of 3% to 35%, some studies reported an increase of enamel porosity, a
loss of mineral content, and a loss of prismatic form(12,13)plus a substantial reduction
in resin composite bond strength.(14,15)On the other hand, Sterrett et al(16)and Haywood
et al(17,18)found no alteration on enamel except normal morphologic variations. Many
found no adverse effect of bleaching on bond strengths of orthodontic brackets, although many others(5,14,15,22)have reported a significant reduction in bond strength after dental bleaching.
• The purpose of this in vitro study is to evaluate the effects of at-home and
in-office bleaching agents on the shear bond strength of metal, ceramic and composite orthodontic brackets; and to compare with unbleached control group.
• Comparison of shear bond strength of metal, ceramic and composite brackets
agents using a Universal Testing Machine (Instron) after bleaching with at-home and in-office bleaching.
• Scanning electron microscopy (using gold sputter coating technique) of
6 Buonocore (1955) outlined a simple method of increasing the adhesion of filling materials to enamel surfaces. He employed 85% phosphoric acid and phosphomolybdate oxalic acid treatment to alter the enamel surface chemically and concluded that phosphoric acid gave better results and was simpler to use.(23)
Reynolds (1975) recommended 6 to 8 MPa as reasonable bond strength for orthodontic purposes. However, this suggestion was made over 38 years ago based on a bracket base area of 16 mm2. Since then, there have been recent advances in bracket materials and design, adhesives, computer technology and testing systems.(24)
Zachrisson (1978) stated that the objective of bonding was to get as good a mechanical interlock as possible between enamel & adhesive and evenly distributed etching pattern with marked surface roughness, but little actual loss of enamel is most desirable to achieve mechanical interlock.(25)
Haywood VB et al (1990) evaluated the effects of 10 % carbamide peroxide bleaching agent on the surface texture of enamel. Bleaching was done on 33 extracted teeth for a period, which would be similar to 5 weeks of night time wear. A control area was made on each tooth and was sealed. After completion of the procedure it was found that there was no difference in colour of treated and control areas. This showed that the colour changing effects extended to portion of the tooth, which was not in contact with bleaching agent as well. No difference in surface texture between treated and control areas were detected.(17)
7 Cvitko E et al in 1991 in his study found that bleaching the enamel with 35 % hydrogen peroxide resulted in surface changes of the enamel and therefore a reduction in bond strength. His study also indicated that at-home bleaching with carbamide peroxide also reduces the shear bond strength of composite to etched enamel. He concluded that removal of surface enamel which was bleached restores the normal bond strength.(27)
Titley KC et al (1991) conducted a scanning electron microscopy observations on the penetration and structure of resin tags in bleached and unbleached bovine enamel at the enamel-resin interface. In the control samples, the resin tags were well defined and contiguous whereas in the 35 % hydrogen peroxide bleached samples, large areas of enamel surface were free of resin. Also the resin tags present were fragmented, ill defined and showed less penetration.(28)
McGuckin RS et al (1992) conducted a study to evaluate the shear bond strength of enamel bond formed at specific time intervals after the Completion of vital bleaching. After bleaching, teeth were bonded at 1, 6 and 24 hours; 3 and 7 days using two different bonding agents and shear bond strength of the specimens were measured. Marked differences among the bleaching treatment, bonding agent and time interval was noted. The interaction between bleaching treatment and time interval was slightly significant other interactions were not significant. It was seen that 80% of bonds failed at the interface or by mixed cohesive composite/ interfacial failure.(29)
8 orthodontic brackets. Samples were divided into 3 groups: Untreated control; enamel treated with 35 % hydrogen peroxide for 2 hours; enamel treated with 10 % carbamide peroxide for 14 days. All the teeth were ground to present a flat surface and cylinders of light cured composite resin were bonded. The mean shear bond strength was found to be less in bleached groups when compared to control group. Therefore it was deducted that bleaching prior to bonding affects the quality of resin-enamel bonds.(30)
Bitter NC (1992) examined the effects of bleaching agent on the enamel surface using scanning electron microscopy. It was revealed that treated enamel had increase surface change and porosity after 30 hours of exposure to bleaching agent. The degree of alteration of enamel surface was not uniform and was influenced by oral hygiene and variation in calcification of different areas.(31)
Seghi RR et al (1992) evaluated the effects of 10 % carbamide peroxide bleaching on indentation and abrasion characteristics of human enamel in vitro. The apparent fracture toughness of enamel reduced by 30 % after bleaching but there was no significant change in surface hardness. There was also a significant decrease in abrasion resistance. It was most likely due to alteration of the organic matrix of enamel.(32)
9 Bishara SE et al in 1993 concluded that bleaching of teeth with 10 % carbamide peroxide did not cause significant effect on the shear bond strength of orthodontic brackets. They mentioned that There is still controversy on the exact nature on how the bleaching products work and what actually happens to the morphology and structure of the enamel surface.(20)
Peter GM et al (1994) did a study to see whether the use of carbamide peroxide (at-home) bleaching agent affected the tensile strength of adhesive pre coated ceramic brackets. 3 groups were made; one was control group, second one was immersed in bleaching agent for 72 hours before bonding and the third one was bleached for 72 hours and stored in distilled water for a week. They suggested that if a patient is using a bleaching agent on his teeth, they discontinue its use at least a week before bonding of orthodontic brackets.(34)
Miles PG et al (1994) conducted a study to investigate the effect of carbamide peroxide at-home bleach on the tensile strength of adhesive pre coated ceramic brackets. They suggested that if a patient is using home bleaching, he should avert from bleaching procedure for at least a week.(14)
10 month. Scanning electron microscope study also showed an apparent decrease in the number of resin tags at the enamel/composite interface for the group bonded immediately post bleaching. They concluded that polymerization inhibition of the resin bonding agent is the likely mechanism for the effects of bleaching on the shear bond strength.(35)
Wasundhara A et al (1995) conducted a study to detect the etching pattern with scanning electron microscopy and the shear bond strength with a Hounsefield tensometer by using 37% and 5% phosphoric acid. It was observed that with 5% phosphoric acid there was minimal enamel loss compared with 37% phosphoric acid. There was no significant difference in shear bond strength, when enamel surface etching was done with 5% and 37% phosphoric acid.(36)
Ben-Amar A et al (1995) evaluated the effect of 10 % carbamide peroxide in a mouthguard on the morphology of enamel surface and shear bond strength of composite resin to bleached enamel surface. The groups were divided into control and test groups. Test group was treated with opalescence bleaching gel using plastic trays and incubated at 37 degrees for 8 hours. Control group was just treated with water soaked cotton. It was found that bleaching created some enamel porosity and significant shear bond strength reduction.(37)
11 bleaching process resulted in a loss of mineral from enamel, which was evident 24 hrs after bleaching and was sustained following 12 weeks storage in artificial saliva. SEM picture showed that there was a definite change in the texture of the bleached enamel surface. Acid etching of the bleached enamel surface produced loss of prismatic form and the enamel appeared over etched. The mean shear bond strength tended to be lower for bleached enamel surfaces. Although surface changes were observed in the etched enamel, the shear bond strength of composite resin luting cement to bleached and etched enamel appeared to be clinically acceptable for delayed bonding.(38)
Ernst CP et al (1996) demonstrated no or slight morphologic changes of enamel surfaces exposed in vitro to four different bleaching agents that contained 10% carbamide peroxide or 30% hydrogen peroxide. In this study, ten freshly extracted, non carious human maxillary incisors were separated into six enamel specimens. Four of these enamel specimens were exposed to different bleaching agents: Opalescence at- home bleaching agent of 10% carbamide peroxide (Ultradent) (exposure time: 6 hours): HiLite, 30% hydrogen peroxide (Shofu Dental) (exposure time: 10 minutes); 30% hydrogen peroxide (exposed for 30 minutes); and 30% hydrogen peroxide mixed with sodium perborate (in a 1:1 ratio) (exposed for 30 minutes). Two specimens were used as positive and negative control: one specimen was treated with 37% phosphoric acid (to provide a relative value for an aggressive solution) and the other was left untreated. All specimens were observed under scanning electron microscopy. The specimens exposed to the bleaching agents revealed no or slight alterations to surface enamel when compared to the control.(39)
12 exposed to carbamide peroxide lost on an average of 1.06 micrograms/mm2 of calcium. The amount of calcium lost was comparable to calcium loss when teeth are exposed to coal beverage for 2.5 minutes. So the amount of calcium loss was not clinically significant.(40)
Rotstein I et al (1996) did a histochemical analysis of dental hard tissues following bleaching. It was found that post bleaching with hydrogen peroxide, there was significant reduction in the calcium/ phosphorus ratio in enamel.(41)
Kugel G et al (1997) recommended the simultaneous use of at-home and in-office systems to bleach teeth, because the combination increased the effectiveness of tooth whitening. Currently there is no study that reports the effect of this technique on shear bond strength.(42)
According to Stanford et al (1997), bond testing using teeth involves many variables that can affect the measured bond strength these variables may include the type of tooth (incisor, premolar, molar, human, bovine); fluoride content of tooth; disinfection and storage media of tooth before bonding; elapsed time of storage following debonding; type of loading (shear, tension, peel, or torsion); configuration of specimen testing jig; crosshead speed of mechanical testing machine; bonding area of the bracket. He suggested that data from different studies must be interpreted carefully and one must consider other factors.(43)
13 variation (standard deviation/mean) in the range of 20% to 30%.(44)
Hegedus C et al (1999) presented an atomic force microscopic study, which evaluated the effect of bleaching agents in enamel surface. The study revealed that home – use bleaching agents are capable of causing enamel surface alterations. Peroxides due to their low molecular weight can penetrate the enamel and may cause its oxidative effects on the inner surface where more organic material is present along with oxidative effects on the outer surface and outer enamel.(45)
Spyrides et al (2000) suggested that the amount of residual oxygen on the bleached enamel surface was reported to have a negative influence on polymerization of the bonding agent. They suggest delaying bonding orthodontic brackets until two weeks after bleaching.(46)
Oltu U et al (2000) evaluated the effects of three concentration of carbamide peroxide on the structure of enamel. 10, 16 and 35 % concentrations were used. It was revealed that 10 and 16 % carbamide peroxide did not affect the structure of enamel, whereas 35 % caused significant changes on enamel structure.(47)
14 Cavalli V et al (2001) performed an in vitro study to determine the effect of elapsed time following bleaching on enamel bond strength of composite resin. 16 groups (n = 12) were used in the study. It was treated with 4 different concentrations of carbamide peroxide at – home bleach and different time intervals of one day, one week, two weeks and 3 weeks post bleaching. Bleach was applied for 6 hours per day for 10 consecutive days. Samples were stored in artificial saliva. For the first 2 weeks after the bleaching procedure, the shear bond strength of resin to enamel was found to be low. But after 3 weeks, the values returned back to normal, similar to untreated control group irrespective of the concentration of the bleaching agent used.(49)
Lai SC et al (2002) hypothesized that bond strength of bleached enamel can be reversed with an anti-oxidant, sodium ascorbate. The hypothesis was later confirmed and sodium ascorbate did reverse the bond strength. He also mentioned that reduction of bond strength in bleached enamel was likely to be caused by the delayed release of oxygen which affected the polymerization of resin components.(50)
Zekonis et al in 2003 did a 3 month single blind study to compare the effects of at home and in office bleaching. Majority, about 84 % of the patients reported at home bleaching treatment to be more effective; 16 % found no difference and none of the subjects found in office bleaching to be superior. There was no difference in tooth sensitivity reported. Gingival inflammation was statistically significantly more in at home bleaching during the end of first week.(51)
15 orthodontic brackets significantly. In bleached group failure occurred more at adhesive/ enamel interface or with in the adhesive unlike in the controlled group where failure occurred at bracket/ adhesive interface.(52)
Shinohara MS et al (2004) evaluated the effect of non vital bleaching on the shear bond strength of composite resin using three different adhesive systems. Bleaching agents used were sodium perborate and carbamide peroxide. After bleaching, the teeth in each group were cut into enamel and dentin sections. The substrates received three different adhesive namely Single Bond (solvent: alcohol/ water); Prime & Bond NT (solvent: acetone), Clearfil SE Bond (solvent: water). The results inferred that bleaching treatment influenced the shear bond strength, regardless of the adhesive system used showing reduction in shear bond strength values. On dentin, the sodium perborate bleaching agent reduced the shear bond strength values, but the carbamide peroxide bleaching did not. They inferred that non vital bleaching treatment with sodium perborate might adversely affect shear bond strength of composite resin for both enamel and dentin. Similar effects can be expected from 37% carbamide peroxide bleaching agent on enamel but not dentin, and the use of water/alcohol and acetone-based adhesive systems cannot reverse the effects of bleaching treatment on bond strengths.(53)
Turkun M et al (2002) conducted a scanning electron microscopy study to investigate the effect of two commercially available 10% carbamide peroxide
16 of bleaching agent and duration of application time. But, these alterations reversed to normal within 3 months.(54)
Pinto CF et al (2004) conducted a study to evaluate the changes in microhardness, surface roughness and morphology of human enamel exposed to 6 different bleaching agents. Bleaching agents were applied according to manufacturers recommendations. Control group was unbleached and stored in artificial saliva. Results showed a significant reduction in microhardness and an increase in surface roughness after bleaching. Enamel morphology was observed under SEM and the changes were noted.(55)
An in vitro study by Basting RT et al (2004), evaluated the shear bond strength of enamel treated with different concentrations of carbamide peroxide (10-22%; 8hours/ day for 42 days) and a placebo to an adhesive system after a post bleaching period of storage in artificial saliva for 15 days. They concluded that after 15 days storage in artificial saliva, different concentrations of carbamide peroxide bleaching agents and a placebo agent had the same enamel shear bond strength values.(56)
Sulieman M et al (2004) investigated the safety of usage of high
concentration of hydrogen peroxide on enamel and dentin. It was observed that there was no evidence of deleterious effects on enamel or dentine. So they concluded that it must be assumed that studies which reported adverse effects on enamel and or dentine of bleaches reflect not the bleach itself but the pH of the formulation used.(57)
17 ceramic brackets. Ceramic brackets being harder than enamel can cause abrasion of opposing teeth. In such cases polycarbonate brackets may be used. He also mentions the importance of sticking to the manufacturer’s guidelines during debonding of
SE Bishara et al (2005) conducted a study to determine the effect of enamel bleaching on the shear bond strength of orthodontic brackets bonded with a composite adhesive. 10 % carbamide peroxide and 25 % hydrogen peroxide were used in the study and the samples were stored in artificial saliva. The results showed that in-office and at-home bleaching did not affect the shear bond strength of orthodontic brackets to enamel. They also found that the enamel surface appeared mildly etched after bleaching in both techniques. After the bleached enamel was etched with 37% phosphoric acid they showed that the honeycomb pattern was irregular in both procedures. This effect was more apparent with in- office bleaching than at- home bleaching regimen.(21)
Miranda CB et al (2005) conducted an inviro study to evaluate the qualitative effect of bleaching agents on the surface morphology of human enamel using SEM. 35 % carbamide peroxide and 35 % hydrogen peroxide were used in the study. Morphological alterations were similar with both the agents. Surface porosities, depression areas, craters and exposure of enamel rods could be detected. They noticed that enamel damage was randomly distributed and the degree of damage also varied randomly.(58)
18 months. Out of them, 58 patients were satisfied. It was concluded that in-office bleaching may be used in patients who do not prefer home bleaching. In-office treatment can achieve satisfactory results, but may require multiple visits.(59)
H Bulut et al in 2006 did a study to investigate the effect of antioxidant and delayed bonding on shear bond strength of metal brackets bonded with composite resin to human enamel after at-home bleach with carbamide peroxide. It was concluded that bonding immediately after at-home bleaching with 10 % carbamide peroxide significantly reduces shear bond strength of composite resin to enamel. They also showed that treating the bleached surface with 10 % sodium ascorbate or delaying bonding for a week reverses the reduction in shear bond strength.(60)
Cadenaro M et al (2006) conducted an in vitro study to find out the influence of whitening agents on the degree of conversion of dental adhesives on dentin. He mentioned that polymerization of the adhesive is reduced after dentin whitening and that delayed adhesive application reverses it.(61)
Bistey et al (2007) conducted an invitro study of the effects of hydrogen peroxide on superficial tooth enamel using spectroscopy. It was found that both at-home and in-office bleaching was capable of causing alteration in enamel at both low and high concentrations. Higher concentration and longer treatment times resulted in more severe alterations of enamel surface.(62)
19 Hakan T et al (2007) evaluated the effects of bleaching and desensitizer application on shear bond strengths of orthodontic brackets. It was found that bleaching significantly affected the shear bond strength of orthodontic brackets to enamel and therefore bleaching should be delayed until completion of orthodontic treatment.(64)
Borges AB et al (2007) evaluated the influence of bleaching agents on enamel bond strength of a composite resin according to storage time in artificial saliva. The bond strength values obtained after 3 weeks post bleaching was significantly higher and were similar to that of unbleached group.(65)
Unlu N et al in 2008 investigated the effect of post treatment time on the shear bond strength of composite resin to bleached enamel with 10 % carbamide peroxide and 35 % hydrogen peroxide bleaching systems. From the study it was concluded that waiting 24 hours after 10 % carbamide peroxide bleach is necessary to provide shear bond strength close to unbleached enamel and a waiting period of 1 week is advised when bleached with 35 % hydrogen peroxide.(66)
Nimet U et al (2008) conducted a study to find out the effect of post-treatment time on the shear bond strength of composite resin to human enamel after bleaching
with 10% carbamide peroxide and 35% hydrogen peroxide bleaching agents. It was
found that bonding immediately after bleaching reduced the shear bond strength
values. Also exposure to artificial saliva reversed the shear bond strength values
towards normal. So its recommended to wait 24 hours after 10% carbamide peroxide
bleaching and 1 week after 35 % hydrogen peroxide bleaching.(67)
20 strength of composite resin with sound enamel and dentin. They recommended a delay of 7 days before attempting any restorative procedures on enamel.(68)
Virna CP et al (2009) conducted an in vitro study to evaluate the bond strength of metallic brackets after dental bleaching. The bleaching agents used were 10 % carbamide peroxide and 35 % hydrogen peroxide. The null hypothesis of the study was that there is no difference between the action of at home and in office bleaching on the shear bond strength of metallic brackets bonded with composite resin 24 hours post bleaching. It was later concluded that use of 35 % hydrogen peroxide bleaching significantly reduced the shear bond strength values and also reduced the amount of resin remnant on the tooth surface after bracket debonding whereas use of 10 % carbamide peroxide did not significantly affect the shear bond strength.(69)
Michel G et al (2009) reviewed the adverse and undesirable effects of tooth whitening agents. It was mentioned that hydrogen peroxide which is a strong oxidizing agent may produce some local undesirable adverse effects. Mechanism of bleaching involves the degradation of the extracellular matrix and oxidation of chromophores present in the enamel and dentin. The local effects include pulp sensitivity, cervical resorption, release of some components from restorations and alteration of enamel surface. It was also mentioned that most of the adverse effects depend on the technique and concentration of the material used and they never generate any acute toxic effects. Neither does carcinogenicity or genotoxicity occurred at concentrations used for dental procedures.(70)
21 teeth. 38 patients were involved in the study and they used a split mouth technique with one arch exposed to in-office bleaching with 38 % hydrogen peroxide while the other arch served as control. Patients were divided into 2 groups. Brackets bonded within 24 hours of bleaching and 2-3 weeks after bleaching. The study revealed that brackets bonded with in 24 hours have a significantly higher chance for bond failure. They recommend that orthodontic bonding should be delayed for 2-3 weeks if patients have a history of in-office bleaching.(71)
Wiltshire et al (2010) mentioned that debonding force is determined from the load drop on the mechanical machine and reported in units of Newtons (N), kilogram (kg), or pounds (lb). Bond strength is defined as the force of debonding divided by the area of the bonded interface measured in units of megapascals (MPa), kilograms per square centimeter (kg/cm2), pounds per square inch (lb/in2 or psi). It is difficult to estimate the optimal bond strength of an adhesive in the oral environment. This is because the orthodontic brackets are subjected to masticatory forces, which are often a mixture of shear, peel, shear-peel, and tensile force. Rather than focusing on an arbitrary numerical “clinical acceptable bond strength”, they suggested to pay more
attention to potential damage to the enamel, especially when the bond strength is too high. They recommended mean bond strength of at least 3 - 4MPa in vitro for minimal reliable clinical bonding.(72)
22 orthodontic bonding whereas peroxide affected the shear bond strength in a negative manner. Shear bond strength values associated with use of carbamide peroxide was significantly lower and is contraindicated before bracket bonding to enamel.(73)
Rafel BJ et al (2011) conducted an in vitro study to evaluate the effects of external bleaching on the morphology of human enamel. Carbamide peroxide concentrations of 16 % and 22 % were used. Bleaching lasted 8 hours a day, for 2 weeks, with 45 days of interval between sessions. The specimens were kept in artificial saliva at 37° C. The SEM results showed depression areas, irregularities, erosion, and enamel prisms exposition. It was concluded that the excess of bleaching produced many alterations on enamel surface, mainly when used in higher concentration.(74)
Oztaz et al (2012) conducted an invitro study to evaluate the effects of bleaching and delayed bonding on the shear bond strengths of metal and ceramic brackets bonded with light and chemically cure composite resin to human enamel. 120 freshly extracted human premolars were used in the study. It was divided into 3 groups. They indicated that 20 % carbamide peroxide bleaching did not significantly affect the shear bond strength of metal and ceramic orthodontic brackets bonded with chemically or light-cure composite resin to enamel when bonding occurred 24 hours or 14 days after bleaching.(75)
23 He concluded that bleaching should be withheld till the completion of orthodontic treatment as the shear bond strength after intracoronal bleaching was found to be low. He also stated that if at all used, carbamide peroxide should be preferred and least recommended one is sodium perborate.(11)
GC Rodrigues et al in 2013 did an in vitro study to find out if time interval after bleaching influenced the adhesion of orthodontic brackets. They concluded that shear bond strength of unbleached sample was considerably higher than bleached groups. Also it was shown that at home bleached group gave acceptable shear bond strength values. After in office bleaching a three weeks waiting period is recommended.(76)
Ahmet YG et al in 2013 did an in vitro study to determine the effects of different bleaching methods on the shear bond strength of metal brackets to human enamel. It was concluded that even though both bleaching methods – in-office and at-home reduces shear bond strength of orthodontic brackets to enamel, at-at-home bleaching method affected shear bond strength more adversely than in-office method of tooth bleaching.(77)
24 The current study was done after getting approval from Institutional Human Ethics Committee on 26/10/2014, Ref. No. SMIMS/IHEC/2014/A/21. The following study was done at the Department of Orthodontics, Sree Mookambika Institute of Dental Sciences, Kulasekharam and Sree Chitra Tirunal Institute For Medical Sciences And Technology - Biomedical Technology Wing, Poojappura, Thiruvananthapuram. The following materials, instruments and equipments were used during the study. Approximate total duration of study was one month.
1) Ninety six non carious extracted human mandibular first premolars.
2) Distilled water.
3) Cold cure Acrylic – Acralyn R (Asian acrylates, Mumbai)
4) Orthodontic lower premolar brackets (MBT 0.022” slot)
1. 3M Unitek: Gemini series metal brackets (119-791, 119-792)
2. American orthodontics: Silkon plus composite brackets (2978MB, 002-2979MB)
3. 3M Unitek: Gemini clear ceramic brackets (117-311, 117-312)
5) Protec Prophylaxis paste
6) 37 % phosphoric acid (D tech)
7) Bracket holder
8) MBT guage
25 10)Transbond XT Primer (3M Unitek. 712 - 034) - Monorovia , CA
11)Opalescence bleaching system – At-home: Opalascence non PF (Ultradent, South Jordan, Utah)
12)Opalescence bleaching system – In-office: Opalescence Boost PF (Ultradent, South Jordan, Utah
1) Sputter coater (Hitachi E 1010 ion sputter)
2) Scanning Electron Microscope (Hitachi S 2400, SEM)
3) Visible light curing unit (Woodpecker LED D Light cure unit, DC-5.0V) 4) Universal testing machine, (INSTRON model-3345)
Detailed description of the test groups:
Groups Number code colour
Subgroups Sample size
Bleaching agent used
Group I a 10 Metal
Group I Black Group Ib 10 None Ceramic
Group Ic 10 Composite
Group IIa 10 Metal
Group II Blue Group IIb 10 At- home Ceramic
Group IIc 10 Composite
Group IIIa 10 Metal
Group III Red Group IIIb 10 In-Office Ceramic
In this study a total of 96 human extracted teeth are required which include the teeth needed for Scanning Electron Microscopy (SEM) studies.
Scientific basis of sample size used in study:
Based on the formula (2pq x 7.84) / (p1-p2)2; where p1 & p2 are the proportion/mean/percentage of any one group, p = (p1+ p2) / 2.
Inclusion criteria: Premolar teeth extracted for orthodontic purpose
Grossly decayed or fractured teeth
Teeth with restoration on buccal surface
Previously bleached teeth
Previously bonded teeth
Any remaining soft tissue was removed with dental scaler and the teeth were stored in distilled water at room temperature.
Scanning Electron Microscopy (SEM)
Six extracted human lower premolar teeth were used for the study. Enamel surface morphology was examined at 1500x and 3000x.
Specimen 1: Normal enamel
Specimen 2: It was acid etched with 37 % phosphoric acid for 30 seconds and rinsed with water for thirty seconds.
Specimen 3: It was bleached with at-home bleach for 8 hours a day for 14 days and rinsed for thirty seconds with water every day after bleaching.
Specimen 4: It was bleached with in-office bleach for 20 minutes and rinsed with water for thirty seconds, repeated once the next day.
Specimen 5: It was bleached with at-home bleach for 8 hours a day for 14 days followed by acid etching one day later with 37 % phosphoric acid for 30 seconds and rinsed with water for thirty seconds.
Specimen 6: It was bleached with in-office bleach for 20 minutes and rinsed with water for thirty seconds, repeated once the next day. It was subjected to acid etching a day later with 37 % phosphoric acid for 30 seconds and rinsed with water for thirty seconds.
Procedure in detail
Teeth were to be divided into 3 groups of 30 each. Teeth were mounted vertically in self cure acrylic resin block so that the crown portion alone was exposed. The teeth were mounted on acrylic blocks such that the roots were completely embedded in the acrylic up to the cemento enamel junction leaving only the crown portion exposed. The blocks were coded with coloured numbers black, blue and red respectively for easy identification. The buccal enamel surface was pumiced, washed and dried before bleaching.
For bleaching two agents were used in this study.
1. In-office bleaching using hydrogen peroxide 40 % (Opalescence boost PF)
2. At-home bleach using carbamide peroxide 10% (Opalescence non PF)
Each group was sub divided into 3 sub groups of 10 teeth.
Group Ia, Ib, Ic are control groups which were not bleached.
Groups IIa, IIb, IIc are bleached using at-home bleaching method
Groups IIIa, IIIb, IIIc are bleached using in-office bleaching method.
29 In-office bleaching was done by applying the bleaching agent directly from the syringe on to the labial surface and was kept undisturbed for 20 minutes. Then the teeth were washed and stored in distilled water. The process was repeated again the next day.
After both types of bleaching, teeth are stored in distilled water for 24 hours before bonding.
Then Groups Ia, IIa, IIIa are bonded with 3m Gemini metal brackets, Ib, IIb, IIIb with 3m Gemini clear ceramic brackets and Ic, IIc, IIIc bonded with Silkon plus (American Orthodontics) composite brackets.
Shear bond strength testing
After completion of bonding protocols the specimens were then subjected to shear bond strength test using Universal Testing Machine (Instron machine, 3345). The machine consists of two jigs. The upper jig was attached to the moving element of the machine cross head element. The immovable part was attached to the lower jig. The crosshead elements were connected to the plotter and the monitor. The teeth mounted vertically on the acrylic block, were carefully oriented in the jig in order to maintain distance and parallel orientation of the labial surface of the tooth and the shearing die. The shear force at a crosshead speed of 1 mm/minute was transmitted to the bracket by a chisel edge blade. The blade was custom made approximately the same size as the bracket edge. The force required to shear the bracket causing bonding failure was recorded in Newtons and the bond strengths were calculated in MegaPascals.
The test was repeated on all the samples and the values obtained were recorded. The data was stored on PC using the software Origin 6.1, Origin Lab, California, USA and the readings of shear bond strengths were recorded in Newtons were converted into Megapascals.
Shear bond strength in megapascals = Debonding force in Newton Bracket base area in mm2
Figure 1: Premolars mounted in acrylic blocks
Figure 4: Group I samples – control
Figure 6: Group III samples for in-office bleaching
Figure 8: Application of at-home bleaching
Figure 10: Group III samples after application of in-office bleaching agent agent
Figure12: Sputter coating unit
Figure 14: Group I after bonding
Figure 16: Group III after bonding
Figure 18: Cross head used for shear bond strength testing (frontal view)
31 The purpose of this study was to determine the effects at home and in office bleaching on the shear bond strengths of metal, composite and ceramic brackets bonded with light cure composite material to human enamel and to compare the shear bond strengths of metal, ceramic and composite brackets after at-home and in-office bleaching. Descriptive statistics, including the mean, standard deviation, and minimum and maximum values, were calculated for each group. The data is expressed in MEAN ± SD. Statistical Package for Social Sciences (SPSS 16.0) version was used for statistical analysis. One way ANOVA was applied for analysis. Post Hoc followed by Dunnet t test was used to find statistical significance between and within the groups. P value less than 0.05 (P<0.05) considered statistically significant at 95% confidence interval.
The mean shear bond strength of metal brackets in control group (Ia) was found to be 16.03±0.87 MPa. It decreased to 14.68±1.67 MPa in the at-home bleached (IIa) group and reduced further to 10.95±2.61 MPa in the in-office bleached group (IIIa). The mean shear bond strength of ceramic brackets in control group (Ib) was found to be 20.21±0.94 MPa. It decreased to 18.31±1.23 MPa in the at-home bleached (IIb) group and reduced further to 16.13±2.67 MPa in the in-office bleached group (IIIb). The mean shear bond strength of composite brackets in control group (Ic) was found to be 9.81±0.61 MPa. It decreased to 8.06±1.88 MPa in the at-home bleached (IIc) group and reduced further to 7.22±2.15 MPa in the in-office bleached group (IIIc).
32 There was significant difference (p<0.05) between group II (at home) and Group III (in office) except in case of use of composite brackets. Also there was intra group statistical significance (p<0.05) in the mean shear bond strength values among metal, ceramic and composite brackets in groups I, II and III. The highest values for SBS were measured in group Ib (20.21±0.94 MPa). The lowest values for SBS were measured in group IIIc (7.22±2.15 MPa). Detailed descriptions of the results are provided in the tables 1 – 12.
Scanning Electron Microscopic Study
Specimen 1 (Normal enamel): Sound enamel surface indicating no alterations. (Figure: 20, 21)
Specimen 2 (Etched with 37 % phosphoric acid for 30 seconds): Shows type I etching pattern with honeycomb appearance. (Figure: 22, 23)
Specimen 3 (Bleached with at home bleach): Showed alterations on surface smoothness and presented different levels of surface changes. Minor changes of the enamel surface occurred in samples treated with 10% carbamide peroxide for 8 hours daily for 14 days. This aspect suggested an insignificant increase in the enamel porosity, as compared to the control samples. Mild surface erosion and depressions were some of the other noted alterations. (Figure: 24, 25)
33 could also be observed. (Figure: 26,27)
Specimen 5 (At home bleach followed by etching with 37 % phosphoric acid): Honeycomb appearance is seen even though pattern is not uniform. Some of the pores appear clogged. (Figure: 28,29)
Table-1: Shear bond strength (MPa) values of different sample of group-I Sample number Group-I a Group-I b Group-I c
1 16.32 21.74 10.93
2 15.38 21.93 9.15
3 15.41 18.94 9.80
4 17.56 19.45 9.24
5 15.34 20.45 10.45
6 16.93 19.00 10.95
7 15.03 20.76 10.34
8 16.78 19.32 9.23
9 15.24 20.56 9.25
10 16.34 19.92 9.89
Table-2: Shear bond strength (MPa) values of different sample of group-II Sample number Group-II a Group-II b Group-II c
1 14.67 17.91 6.94
2 15.89 19.34 9.32
3 17.45 18.34 8.45
4 11.67 19.23 9.42
5 13.97 20.14 7.45
6 14.00 17.34 8.45
7 16.34 16.03 7.24
8 15.12 19.23 8.12
9 13.04 18.34 8.04
10 14.67 17.23 7.19
Table-3: Shear bond strength (MPa) values of different sample of group-III Sample number Group-III a Group-III b Group-III c
1 10.61 15.91 7.09
2 12.90 18.09 7.29
3 10.32 20.89 11.45
4 11.73 16.45 7.56
5 10.79 14.89 5.12
6 11.34 15.67 7.34
7 14.92 19.45 6.03
8 5.23 14.23 10.02
9 12.78 13.19 4.34
10 8.89 12.56 6.00
(MEAN±SD) 10.95±2.61 16.13±2.67 7.22±2.15 Table-4: Mean values of shear bond strength (MPa) of group-I
Group-I Type of bracket Shear bond strength (MPa) (MEAN±SD)
Group-I a Metal 16.03±0.87
Group-I b Ceramic 20.21±0.94
Table-5: Mean values of shear bond strength (MPa) of group-II Group-II Type of bracket Shear bond strength (MPa)
(MEAN±SD) Group-II a Metal 14.68±1.67
Group-II b Ceramic 18.31±1.23
Group-II c Composite 8.06±1.88
Table-6: Mean values of shear bond strength (MPa) of group-III Group-III Type of bracket Shear bond strength (MPa)
(MEAN±SD) Group-III a Metal 10.95±2.61
Group-III b Ceramic 16.13±2.67
Group-III c Composite 7.22±2.15
Table-7: Multiple comparison of mean value of shear bond strength (MPa) within the group-I
Group-I Shear bond strength (MPa) (MEAN±SD)
P value Group-I a 16.03±0.87 G-I a with I b 0.001
G-I a with I c 0.001
Group-I b 20.21±0.94* G-I b with I c 0.001
Group-I c 9.81±0.61*,#
Table-8: Multiple comparison of mean value of shear bond strength (MPa) within the group-II
Group-II Shear bond strength (MPa) (MEAN±SD)
P value Group-II a 14.68±1.67 G-II a with II b 0.001
G-II a with II c 0.001
Group-II b 18.31±1.23* G-II b with II c 0.001
Group-II c 8.06±1.88*,#
(*P<0.05 significant compared group- IIa with IIb and IIc, #P<0.05 significant compared group- IIb with IIc)
Table-9: Multiple comparison of mean value of shear bond strength (MPa) within the group-III
Group-III Shear bond strength (MPa) (MEAN±SD)
P value Group-III a 10.95±2.61 G-III a with III b 0.001
G-III a with III c 0.009
Group-III b 16.13±2.67* G-III b with III c 0.001
Group-III c 7.22±2.15*,#
Table-10: Multiple comparisons of mean value of shear bond strength (MPa) of different groups
Groups Shear bond strength (MPa) (MEAN±SD)
Groups comparison P value Group-I a 16.03±0.87 G-I a with G-II a 0.282
G-I a with G-III a 0.001
Group-II a 14.68±1.67 G-II a with G-III a 0.001
Group-III a 10.95±2.61*,#
(*P<0.05 significant compared group-I a with III a, #P<0.05 significant compared group-II a with III a, P>0.05 no significant compared group-I a with II a)
Table-11: Multiple comparisons of mean value of shear bond strength (MPa) of different groups
Groups Shear bond strength (MPa) (MEAN±SD)
Groups comparison P value Group-I b 20.21±0.94 G-I b with G-II b 0.082
G- I b with G-III b 0.001
Group-II b 18.31±1.23 G- II b with G-III b 0.04
Group-III b 16.13±2.67*,#
Table-12: Multiple comparisons of mean value of shear bond strength (MPa) of different groups
Groups Shear bond strength (MPa)(MEAN±SD)
Groups comparison P value Group-I c 9.81±0.61 G-I c with G-II c 0.22
G-I c with G-III c 0.001
Group-II c 8.06±1.88 G-II c with G-III c 0.419
Group-III c 7.22±2.15*
Figure 20: Normal enamel surface (1500X)
Figure 22: 37 % Phosphoric acid etched enamel surface (1500X)
Figure 24: At-home bleached enamel surface (1500X)
Figure 26: In-office bleached enamel surface (1500X)
Figure 28: Etched enamel surface after at-home bleaching (1500X)
Figure 30: Etched enamel surface after in-office bleaching (1500X)
Graph-1: Mean values of shear bond strength (MPa) of group-I
Group I - Control group: Group Ia – Metal bracket, group Ib – Ceramic bracket, group Ic – Composite bracket
Graph-2: Mean values of shear bond strength (MPa) of group-II
Graph-3: Mean values of shear bond strength (MPa) of group-III
Group III – In-office bleached group: Group IIIa – Metal bracket, group IIIb – Ceramic bracket, group IIIc – Composite bracket
Graph-4: Multiple comparisons of mean value of shear bond strength (MPa) of different groups
Graph-5: Multiple comparisons of mean value of shear bond strength (MPa) of different groups
Group Ib - Control group, group IIb – At-home bleached group, group IIIb – In-office bleached group (Ceramic brackets)
Graph-6: Multiple comparisons of mean value of shear bond strength (MPa) of different groups
41 The basis for the adhesion of brackets to enamel has been enamel etching with phosphoric acid, as first proposed by Buonocore in 1955.(23) Achieving a low bond failure rate should be a high priority objective, since replacing loose brackets is inefficient, time-consuming, and costly.(79) The adhesion of composite resin to tooth enamel is provided principally by the mechanical bonding in which the unfilled phase of resin system penetrates and polymerizes in irregularities induced in the enamel surface. The surface penetration of the resin is enhanced by treating the enamel with an acid such as 37% phosphoric acid that selectively demineralizes the enamel creates micropores in its surface, and significantly increases the surface area and its wettability.
There is an 800% increase of adult patients in the United States receiving orthodontic treatment from 1970 to 2003. The actual number of adults having orthodontic therapy probably has increased and has the potential to increase even further as more sophisticated and aesthetic methods of treatment are used.(80) Patients who visit an orthodontic clinic have esthetic concerns. Therefore, both tooth appearance and color is important to them.
42 is scheduled 24 hours after completion of bleaching procedure.
Some adverse effects of vital bleaching are sensitivity, gingival irritation, ulcers, compromised bond strength of composite resin and reversal of color. In the instant life style the compromised bond strength of resin composites to teeth, after bleaching is of more clinical concern. The prolonged periods of postponing the bonding procedures would increase the patient’s anxiety.
The technique of bleaching or whitening teeth was first described in 1877 by Chapple. Since then bleaching of teeth has been in use with little change in science or technique during that time.(81) In-office bleaching was never very popular because of the danger to the patient and the dentist, the amount of time it took to do it, and the cost to the patient. The danger to the patient is the potential for tissue burns from the high concentration of hydrogen peroxide used, which can result from a leaky rubber dam or improper isolation technique. There are also some questions related to dangers to the pulp due to certain lights used and the heat generated.(81) With the introduction of home bleaching tooth whitening has regained great popularity and reached the more people in population.
Although process of in-office bleaching and at-home bleaching are different, they are based on hydrogen peroxide as an active agent for bleaching. However, concentrations of hydrogen peroxide in home bleaching and in-office bleaching are different. While a 10% carbamide peroxide bleaching product contains 7% urea and 3% hydrogen peroxide, an in-office bleaching product contains about 35% hydrogen peroxide.(81)
43 ability of hydrogen peroxide to form oxygen free radicals that interact with colored organic molecules and oxidize these macromolecules and pigment stains, which produce dental discoloration into smaller and lighter molecules.(49)
The urea in carbamide peroxide primarily acts as a stabilizer to give these products a longer shelf life, slower release of the hydrogen peroxide, and it has additional cariostatic benefits. Hydrogen peroxide penetrates the tooth more quickly than carbamide peroxide. The basic mechanism of action is the same, but the formulation affects shelf life and time required for penetration of the tooth.(82)
Carbamide peroxide dissociates into hydrogen peroxide and urea when in contact with soft-tissues or saliva at oral temperatures.(49) The resulting hydrogen peroxide then ionizes. On the other hand, urea degrades into ammonia and carbon dioxide.(35)
Many(27,30,33,53,60,67,75-77) studies have shown that the various bleaching methods have adversely affected the shear bond strength of orthodontic brackets to enamel. The current study was done to find out the effect of at-home and in-office bleaching procedures on the shear bond strength of metal, ceramic and composite brackets to enamel.
44 agent by ADA.(17,20,39) On the other hand, contrary results have shown the morphological alterations on enamel surface bleached with 10% carbamide peroxide.(32,47)
In the current study, the effect of at home and in office bleach on the enamel surface morphology was studied using SEM. It was found that at home bleaching resulted in an insignificant increase in the enamel porosity, as compared to the control samples. Mild surface erosion, depressions, and increased depth of enamel grooves were some of the other noted alterations. This was in agreement with other studies.(35,38,46)
In the present study there was significant difference (p<0.05) in the bond strengths of group I (control) and group III (in office bleached). SEM analysis revealed that in-office bleaching resulted in surface alterations and intense surface deposits. Morphologic surface alterations became much more pronounced after in office bleaching. Intermittent depressions of various depths were present; craters and shallow erosions could also be observed. These observations were in agreement with other studies.(21,27,58)